International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 05 Issue: 06  June2018
pISSN: 23950072
www.irjet.net
EFFECT OF PROCESS PARAMETERS ON MECHANICAL PROPERTIES OF LASER BEAM WELDED JOINTS B.Govardhan1, P. Rama Murty Raju2, S.Rajesh3 M. Tech. (CAD/CAM) PG student, S.R.K.R Engineering College, Bhimavaram534204 Department of mechanical engineering, S.R.K.R. Engineering College Bhimavaram534 204 3Associate Professor, Department of mechanical engineering, S.R.K.R. Engineering College Bhimavaram534 204 ***1
2Professor,
for joining dissimilar and nonmetallic materials, and for creating products of innovative shapes and designs. Lot of researchers are investigation to deal with the estimation of weld bead geometry, Heat affected zone, hardness and microstructure. Balasubramaniam (1) Investigated that beam power and weld speed are major process parameters influencing on depth of penetration and bead width. This thesis tries to clarify the various background issues concerning the laser beam welding of stainless steels.Codigo Do Tradalho (2) has carried out investigation to weld joint gap on 304L stainless steel using CO2 laser welded joints to characterize weld bead geometry.
AbstractIn the present study stainless steel material 304
grade was chosen for joining using laser beam welding process. Tensile strength and bending strength are considered as output responses. Empirical modeling of output responses in terms of process parameters is established and the effect of process parameters on the output variables has been studied. The effect of each parameter has been studied. Analysis of Variance (ANOVA) has been used for finding the contribution of each factor on the output parameters. The main effects plots and the interaction effect plots have been plotted in order to understand the actual effect of input on the output. The responses have been predicted by regression analysis using MINITAB..
2. Literature Review
Keywords: ANOVA, CO2 laser welding, MINITAB.
Alexandra et.al (2003) has worked on laser beam welding hard metals to steel. They have examined Laser beam weld ability of hard metals to steel with high power (cw) CO2 laser, (cw) Nd: YAG laser and (pw) Nd: YAG laser.
1. INTRODUCTION The acronym “LASER” stands for Light Amplification by Simulated Emission of Radiation is a coherent and amplified beam of electromagnetic radiation. The key element in making a practical laser is the light amplification achieved by stimulated emission due to the incident photons of high energy. Laser comprises of three components namely lasing medium, lasing energy source and optical delivery or feedback system. The laser medium may be a solid, liquid or gas. Laser light differs from ordinary light because it has photons of same frequency, wavelength and phase, laser beams are highly directional, have high power density and better focusing characteristics. Among different types of lasers Nd:YAG and CO2 are most widely used now a day’s. In this process material is joined by focusing highly intense laser beam on the work piece. Welding is a process of joining the surfaces of two workpieces (usually metals) through localized coalescence. It is a precise, reliable, costeffective, and hightech method for joining materials. No other technique is as widely used by manufacturers to join metals and alloys efficiently and to add value to their products. Most of the familiar objects in modern society, from buildings and bridges, to vehicles, computers, and medical devices, could not be produced without the use of welding.
They have deduced that the laser beam welding process has the overall advantage of producing small beads and HAZ and minimizing residual stresses. Continuous Nd: YAG laser was found to present the best results. Ribolla et.al (2005) has investigated the use of Nd: YAG laser weld for large scale volume assembly of automotive body in white. They have suggested some advantages in laser welding as a variety of benefits over other types of welding. Deep penetration of precise narrow welds, small heat affected zone, low heat input, fast weld times, minimum part distortion, no secondary processing and high repeatability can be mentioned as great advantages. Balasubramanian et.al (2006) has worked on Mathematical and ANN Modeling of Nd: YAG laser welding of thin SS Sheets. The effect of laser power (0.61.4 kW), welding speed (0.82 m/min) and shielding gas flow rate (5  15 l/min) on the weldbead geometry i.e. depth of penetration (DOP), weld bead width (BW) was investigated. The experiment was designed on three levels BoxBehnken design with replication. Modeling was done using artificial neural network and multiple regression analysis. Comparison of neural network model and multiple linear regression model was made.
Nowadays, welding goes well beyond the bounds of its simple description. This technique is applied to a wide variety of materials and products, using advanced technologies, such as lasers and plasma arcs. The future of welding holds even greater promise as methods are devised © 2018, IRJET

Impact Factor value: 7.211
Roberto Berrettaa et.al (2007) have investigated the pulsed Nd: YAG laser welding of AISI 304 to AISI 420 
ISO 9001:2008 Certified Journal

Page 2975
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 05 Issue: 06  June2018
pISSN: 23950072
www.irjet.net
stainless steels. They have studied the influence of the laser beam position, with respect to the joint, on weld characteristics. The joints were examined in an optical microscope for cracks, pores and to determine the weld geometry. The microstructure of the weld and the heat affected zones were observed in a scanning electron microscope. Vickers microhardness testing and tensile testing were carried out to determine the mechanical properties of the weld.
Matlab software to establish the relationships between the laser welding input parameters like beam power, travel speed and focal position and the three responses DP, BW and TS in three different shielding gases(Argon, Helium and Nitrogen). Yang dongxia et.al (2012) has worked on Optimization of weld bead geometry in laser welding with filler wire process using Taguchi’s approach. In their work, laser welding with filler wire was successfully applied to joining a newtype Al– Mg alloy. Welding parameters of laser power, welding speed and wire feed rate were carefully selected with the objective of producing a weld joint with the minimum weld bead width and the fusion zone area.
Glowski et.al (2009) have studied the characteristics of Nd: YAG laser welded joints of dual phase steel. They have presented the examination results of microstructure, mechanical properties, fatigue strength and residual stresses of Nd: YAG laser welded joints in dual phase HDT580X steel. They have concluded that the laser welding parameters were appropriate to obtain sound welds. They have indicated that it was possible to achieve good quality welds by the application of proper welding parameters.
This paper aimed to examine the influence of weld speed, power and focusing distance on the welded joint performance. The effect of each parameter has been studied. Analysis of Variance (ANOVA) has been used for finding the contribution of each factor on the output parameters. The main effects plots and the interaction effect plots have been plotted in order to understand the actual effect of input on the output. The responses have been predicted by regression analysis using MINITAB.
Padmanaban et.al (2010) has worked on an optimization of laser beam welding process parameters to attain maximum tensile strength in AZ31B magnesium alloy. An empirical relationship was developed to predict tensile strength of the laser beam welded AZ31B magnesium alloy by incorporating process parameters such as laser power, welding speed and focal position. The experiments were conducted based on a three factor, three level, central composite face centered design matrix with full replications technique. The empirical relationship can be used to predict the tensile strength of laser beam welded AZ31B magnesium alloy joints at 95% confidence level. The results indicate that the welding speed has the greatest influence on tensile strength, followed by laser power and focal position.
3. DESIGN OF EXPERIMENT, EXPERIMENT WORK AND MEASUREMENT This is a non contact process that requires access to the weld zone from one side of the parts being welded. The weld is formed as the intense laser light rapidly heats the material typically calculated in milliseconds. Laser welding is a joining process where laser are used as a heating source for joining the two metal parts. Many advantages of laser welding technology such as high speed and noncontact welding make the use of the technology more attractive in the automotive industry. Quit a number of researchers work has been studied on CO2 laser welding. used 20 kW CO2 laser for welding of mild steel to determine the plasma absorption in the keyhole based on photodiode measurements and spectroscopic measurements. They observed that the plasma absorption of the laser beam can’t neglect in certain welding conditions and plasma studied on the welding of low carbon steel by using the 4KW CO2 laser. The welding parameters were laser power 4KW, welding speed 1.2m/min, shielding gas Helium and Argon its flow rate 11L/min.
Ruggiero et.al (2011) have investigated weldbead profile and costs optimization of the CO2 dissimilar laser welding process of low carbon steel and austenitic steel AISI316. The effect of laser power (1.1–1.43kW), welding speed (25– 75 cm/min) and focal point position ( 0.8 to  0.2 mm) on the weldbead geometry (i.e. weldbead area, A; upper width, Wu; lower width, Wl and middle width, Wm) and on the operating cost C was investigated using response surface methodology (RSM). The results indicate that the proposed models predict the responses adequately within the limits of welding parameters being used. They have used regression equations to find optimum welding conditions for the desired geometric criteria. They have concluded that the welding speed is the parameter that most significantly influences the main weld bead dimensions.
A stainless steel sheet of dimension 1050mm*1050mm*3mm was provided. The sheet was cut in to four small pieces of equal dimension of 100mm*100mm*3mm using LASER cutting machine. The sheet was clamped in the table and then was cut. One of the smaller sheets of equal dimension was taken and the sheet was cut in to small strips of width 1050mm and length 1050 mm. Then these small strips are cut into small plates of dimension 100mm*100mm*3mm. these small sheet are to be welded. After cutting in LASER machine the edges of the small sheets not polished. The surface of the sheets to be
Sathiya et.al (2012) have worked on optimal design for laser beam butt welding process parameter using artificial neural networks and genetic algorithm for super austenitic stainless steel. In that study, the weld bead geometry such as depth of penetration (DP), bead width (BW) and tensile strength (TS) of the laser welded butt joints made of AISI 904L super austenitic stainless steel were investigated. They have developed Artificial Neural networks (ANN) program in © 2018, IRJET

Impact Factor value: 7.211

ISO 9001:2008 Certified Journal

Page 2976
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 05 Issue: 06  June2018
pISSN: 23950072
www.irjet.net
welded should be very smooth. So the surfaces are finished in grinding machine. To remove the bur filing was done. In finishing operation the stainless steel sheet should be continued with very slowly and steadily. So precaution was taken. After converting the big sheets of stainless steel in to small sheets of dimension the small sheets are aligned on the table of the welding machine. The machine used to weld the two sheets of metal.
Figure 2 specimen dimension
3.1 welding process
For bending 200*20*3mm subsamples are machined by using water jet cutting to obtain specified design shape.
Welding takes place by placing two 304L SS material of 100*100*3mm size are first placing both faces to ensure that the joint must in ZEROgap. First operator place the specimen holder with the two specimens to be joined and then pass a low powered LASER beam up on the joint to check the position and direction .spot three high power beam on the joint to ensure that line of direction, after that specified parameters laser beam passed over the specimen for weld and then cool down the welded joint with the help compressed air. Repeat the 9 joints as per given parameter sheet shown in parameter table 1.Figure 1 consist of laser welded joint
Figure 3 Tensile test specimens Tensile test the 200*100 mm laser weld blanks were machined into standard ASTM E8 sheet type sub size transverse weld tensile specimens are shown in fig 3.
Figure1 Laser welded joint
Table 1 Parameter Sheet
The above figure shows LASER beam welded joint specimen the dimension was 200*100*3mm total 9 specimen are prepared
Input Parameters power
The welded samples are machined with water jet cutting to obtain the required sub sample because in this machining HAZ and lubricant are absent which effect on output parameters. As per ASTM E8M standards sample dimensions are chosen for TENSILE test and BENDING test dimensions are given in below fig 2

Impact Factor value: 7.211
Focal
Tensile
Bending
1
speed Strength Strength % of (m/min position (MPa) (MPa) Elongation ) 1700 1.0 (mm) 2 720.6 638 49
2 3
1700 1700
1.5 2.0
0 +2
605.2 596.6
633 403
42 14
4 5
2000 2000
1.5 2.0
2 0
727.8 725.4
643 640
50 50
6
2000
1.0
+2
711.4
635
48
7
2250
2.0
2
741.4
658
53
8
2250
1.0
0
731.9
646
51
9
2250
1.5
+2
731.9
651
52
Exp (W) No.
3.2 sub specimen preparation
ÂŠ 2018, IRJET
Weld
Output Parameters

ISO 9001:2008 Certified Journal

Page 2977
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 05 Issue: 06  June2018
pISSN: 23950072
www.irjet.net
From the table 1, it is identified that the minimum ultimate tensile strength value 596 Mpa is obtained at the value of 1.7 KW Power, 1.0 mm/min travelling speed and +2 mm focal position, zero position length is 200 mm. The maximum ultimate tensile strength value 741 Mpa is obtained at the value of 2.25 KW Power, 2000 mm/min travelling speed and 2 mm focal position.
from the same plot it was observed that tensile strength decreases with the increase in weld speed. This happens as the time for contact between laser beam and work piece decreases then less amount of time period gets to weld it lead poor weld. Tensile strength is decreased with the change in type of laser used. Almost similar pattern was observed with change in weld speed, as depicted in Figure 6, Tensile strength is slightly decreased with increase in focal point.
Figure 4 and 5 shows specimen after testing is tensile tested specimen and bending tested specimen.
LP in kW
WS in m/min
Mean of Tensile Strength in MPa
725
Figure 4 Tensile specimens after testing , Figure 5 Bending specimens after testing
700 675 650 1
Taguchi approach is an effective approach for optimization. There have been plenty of recent applications of Taguchi approach to various mechanical engineering fields for process optimization. Hence, in this work optimization of LBW process parameters and statistical analysis of the experimental data was carried out. Initially Taguchi technique was applied to the L9 orthogonal array experiments in order to identify the optimal values for strength characteristics such as Tensile Strength (TS) and Bending strength (BS) in LBW process. In addition to it linear regression analysis was performed in order to establish a relationship between process parameters and output responses using MINITAB software. Later, ANOVA was performed to observe the parameters which affect significantly the mechanical strength characteristics of LBW joints.
2
3
700 675
2
3
Figure 6 Effect of process parameters on tensile strength
4.1.2 Direct effect of process parameters on bending strength Figure 7 depicts the main effects plots for the means of bending strength values. It indicates the variation of bending strength values with respect to various process parameters. From the Figure 7 it was observed that bending strength increases with the increase in laser power. This indicates that the discharge energy becomes more intense with higher value of laser power. The higher beam discharge energy causes more powerful explosion and deeper welds are formed on the joint. This results in good weld. Hence to obtain good weld bead finish the laser power should be as kept low as possible. On the other hand, low beam power leads to longer welding time required. The individual effect of welding speed on bending strength can be observed from the same plot. The strength increased with the increase in weld speed for certain point after that strength decreased by increasing weld speed, as discharge energy decreases and subsequently deep craters are not formed. Hence, it leads to good weld quality. However, increasing weld speed leads to increasing bending strength for certain point further weld speed increasing causeâ€™s low joining rate. The effect of focal point on bending strength, as seen in same figure, is that hardly any improvement in weld quality is achieved with any lower value of focal point. Similar pattern was observed for weld speed on bending strength. But in weld speed strength was increased for next point and then it decreased at next pint for that certain weld speed was required for good weld.
4.1 Main Effects of Process Parameters on Output Responses 4.1.1 Direct effect of process parameters on Tensile strength Figure 6 shows the main effects plots for the means of tensile strength values. It indicates the variation of tensile strength values with respect to various process parameters. As seen in Figure 6, tensile strength increases with the increase in Laser Power (LP). Increase in laser power increases the level of discharge energy and which subsequently causes more powerful explosion and results in more melting occurs from the work piece. Hence higher values of Laser power leads to greater amount of weld joint efficiency. On the contrary, Impact Factor value: 7.211
1
725
1

3
650
4 Results & Discussion
ÂŠ 2018, IRJET
2 FP in mm

ISO 9001:2008 Certified Journal

Page 2978
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 05 Issue: 06  June2018
pISSN: 23950072
www.irjet.net
Main Effects Plot (data means) for Bending Strength in MPa LP in kW
WS in m/min
Mean of Bending Strength in MPa
650 625 600 575 550 1
2 FP in mm
3
1
2
3
1
2
Focal distance mm
4354
2
2177
Error
3241
2
1620.5
Total
25393
8
1.34
17.14 12.76 100.00
3
650 625 600 575 550
Figure 7 Effect of process parameters on bending strength
4.2 ANOVA for output responses 4.2.1 ANOVA for Tensile Strength In order to investigate the significantly affecting parameters on tensile strength, ANOVA of experimental data was performed for analyzing the influence of laser power (LP); weld speed (WS) and focal point (FP) on the total variance of the results. In addition, the Fisherâ€™s Ftest can also be used to determine the parameters which have a significant effect on the response variable when F is large. The results of ANOVA for tensile strength are shown in Table 2. The last column of the tables indicates the percentage contribution of each factor on the total variation, thus indicating the degree of influence on the tested result. From the analysis of Table 2, it can be observed that the parameters laser power (61.38%) and focal distance (17.14%) influence the tensile strength, whereas the weld speed (8.7%) had lesser then error so no influence on tensile strength. Especially the laser power has greater influence when compared to rest of the factors.
Figure 8 Percentage contributions of process factors on tensile strength Hence in this study, it was found that laser power and focal distance had physical significant effect on the tensile strength.
4.2.2 ANOVA for bending strength Table 3 shows the ANOVA results for bending strength. From this table it can be depicted that parameters laser power (30.06%) and focal distance (24.88%) influence the bending strength, whereas the parameter weld speed (21.20%) had no influence on the bending strength. Especially the laser power has greater influence on bending strength when compared to rest of the factors. The influence of each control parameter on bending strength was represented in Figure 9 graphically. From the ANOVA results, it is clear that the error associated is approximately 23.84% for bending strength. In this study, it was found that laser power have physical significant effect on bending strength.
The influence of each control parameter on tensile strength was represented in Figure 8 graphically. The factors present a physical significance when a percentage of contribution of LP and FP parameter is greater than error associated except weld speed. From the ANOVA results, it is clear that the error associated is approximately 12.76% for tensile strength.
Table 3 Results of the ANOVA for bending strength
Table 2 Results of the ANOVA for tensile strength Predictor
SS
DF
Laser power KW
15587
Weld speed m/min
2211
2
ÂŠ 2018, IRJET

2
Variance
7793.5
1105.5
Fcalculated
4.81
0.68
Predictor
Percentage contribution
SS
DF
Variance
Fcalculated
Percentage contribution
61.38
Laser power KW
15541
2
7770.5
1.26
30.06
8.7
Weld speed 10963 m/min
2
5481.5
0.89
21.20
Impact Factor value: 7.211

ISO 9001:2008 Certified Journal

Page 2979
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 05 Issue: 06  June2018
pISSN: 23950072
Focal distance 12867 mm
2
6433.5
6163
Error
12326
2
Total
51696
8
1.04
www.irjet.net
The adequacy of the models as represented by Equations 1 and 1 are checked using the normal probability plot of residuals for TS and BS as shown in Figure 10 and Figure 11 It can be observed that the points are close to the normal probability line and thus evidencing the model adequacy. Another way of ascertaining about the models adequacy is by plotting the residuals against fitted values of TS and BS. It can be observed that the points representing the residuals are randomly scattered. Thus, the mathematical models formulated for prediction of TS and BS as represented by Equations 1 and 2 are adequate. The values of the TS and BS can be predicted by. Substitute the coded values of the variables in the equation 1 and 2 respectively.
24.88
23.84
100
Residuals Versus the Fitted Values 50
90
25 Residual
Percent
Normal Probability Plot of the Residuals 99
50 10 1
80
40
0 Residual
40
50
80
Histogram of the Residuals
0 25 50
40
20
0 Residual
20
40
1
Normal Probability Plot of the Residuals
2
3
4 5 6 7 Observation Order
8
9
Residuals Versus the Fitted Values 50 Residual
Percent
90 50 10 1
100
50
0 Residual
50
Histogram of the Residuals
500
550
600 Fitted Value
650
700
Residuals Versus the Order of the Data
Residual
Frequency
50
50
1.5 1.0 0.5 0.0
0
100
100
2.0
80
60
40
20 0 Residual
20
40
60
0 50 100
1
2
3
4 5 6 7 Observation Order
8
9
Figure 11 Residual Plots for bending strength
4.4 SNR Analysis of Output Responses In order to evaluate optimal parameter settings, Taguchi method uses a statistical measure of performance called SignaltoNoise Ratio (SNR). The SNR takes both the mean and the variability into account. The SNR is the ratio of the mean (signal) to the SD (noise). The ratio depends on the
BS in MPa = 679+46.8 LP in KW â€“ 36.3 WS in m/min 41.7 FP in mm (Eq. 2) (RSq = 80.9% RSq (adj) = 77.5% Impact Factor value: 7.211
1
99
(RSq = 83.9% RSq (adj) = 78.2%)

760
Figure 10 Residual Plots for Tensile strength
TS in MPa = 688+47.1 LP in KW 16.7 WS in m/min 25.0 FP in mm (Eq. 1)
ÂŠ 2018, IRJET
680 720 Fitted Value
25 Residual
Frequency
Mathematical models for Tensile strength (TS) and bending strength (BS) responses in terms of control variables were developed in the preliminary stage with the regression technique. In the secondary stage Taguchi technique was applied to the L9 orthogonal array experiments in order to identify the optimal values for TS and BS. Using a Minitab version 9 analysis of the influence of each control factors on TS and BS has been performed with SNR response. Experimental layout and their results with calculated SNR for the TS and BS of the composite are furnished in Table 1.8. Considering the TS and BS as response variables and the control factors as inputs, it is possible to develop a mathematical model expressing the relationship between the output and input. The correlations between the main factors and their interactions with TS and BS of the LBW joints were obtained by performing regression analysis. The following Equations 1 and 2 were developed with an RSq 83.9% and 80.9% for TS and BS response variables respectively using method of least squares.
640
Residuals Versus the Order of the Data
2
0
4.3 Regression Analysis of Output Responses
600
50
3
Figure 9 Percentage contributions of process factors on bending strength
0 25

ISO 9001:2008 Certified Journal

Page 2980
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 05 Issue: 06  June2018
pISSN: 23950072
www.irjet.net
quality characteristics of the product/process to be optimized. The standard SNRs generally used are as follows: nominalisbest (NB), lowerthebetter (LB), and higherthebetter (HB). The optimal setting is the parameter combination, which has the highest SNR. In this investigation higherthebetter (HB) is used for TS and lowerthebetter (LB) SNR ratio is employed for BS response functions.
5 Conclusions Experiments were conducted on LBW to evaluate the strength characteristics of 304 stainless steel welded joints .Laser power, welding speed and focal point distance were considered as process parameters while tensile strength and bending strength were considered as output responses. Conclusions derived by application of Regression and Taguchi analysis of experimental results are as follows:
Figure 12 and Figure 13 shows the main effects plots for the TS and BS for SNR mean values. It can be observed form Figures that the greater the SNR, smaller is the variance of the TS around a desired value. It can also be observed that the optimal testing conditions of the control factors can easily be determined. The plot shows the change in SNR when the setting of the control factor was changed form one level to other. The best value is found to be at higher SNR value. From Figures it can also be seen for tested samples the optimum condition for tensile strength becomes LP1 WS1 and FP1 whereas for bending strength the optimum conditions observed are LP1 WS1 and FP1 for main control factors respectively.
Empirical linear regression equations are developed for predicting the bending test errors and tensile test errors respectively within selected experimental conditions. The Taguchi method was applied in order to identify the optimized values of process parameters by taking maximum Tensile strength and maximum bending strength. Based on the ANOVA results for tensile strength, it was depicted that the process parameters, laser power, weld speed and focal point distance have more influence on the strength. In case of bending strength laser power, Focal point exert a significant effect, whereas the parameters weld speed and have less significant effect on the bending strength.
Referances (1) Balasubramanian, K. R., Buvanashekaran, G., Sankaranarayanasamy, K. (2010). Modeling of laser beam welding of stainless steel sheet butt joint using neural networks, CIRP Journal of Manufacturing Science and Technology, Vol. 3, No. 1, 8084 (2) Codigo Do Trabalho: 021018171. (2009). Characterization of Nd:YAG pulsed laser welded austenitic AISI 304L stainless steel, V congresso brasileiro de engenharia de fabricação 14 a 17 de abril de 2009, Belo Horizonte, Minas Gerais, Brasil. Online http://www.ipen.br/biblioteca/2009/eventos/14600.pdf.
Figure 12 SNR Analyses for Tensile Strength
(3) Alexandra, P. Costa, Luisa Quintino, Martin, Greitmann (2003). Laser beam welding hard metals to steel. Journal of Materials Processing Technology 141 163–173. (4) Ribolla, A., Damoulis, G.L., Batalha G.F. (2005). The use of Nd: YAG laser weld for large scale volume assembly of automotive body in white Journal of Materials Processing Technology 164–165 1120–1127. (5) Balasubramanian, K. R., Buvanashekaran G. and Sankaranarayanasamy K. (2006). Mathematical and ANN Modeling of Nd: YAG Laser Welding of Thin SS Sheets. International Journal for the Joining of Materials, Volume 18 No. 3/4 , December 2006, pp 99104. ISSN 09056866. (6) Jose, Roberto Berrettaa and Wagner, de Rossib (2007). The Pulsed Nd: YAG laser welding of AISI 304 to AISI 420 stainless steels / Optics and Lasers in Engineering 45.
Figure 13 SNR Analyses for Bending Strength
© 2018, IRJET

Impact Factor value: 7.211

ISO 9001:2008 Certified Journal

Page 2981
International Research Journal of Engineering and Technology (IRJET)
eISSN: 23950056
Volume: 05 Issue: 06  June2018
pISSN: 23950072
www.irjet.net
960– 966. (7) Wglowski, M.S., Kwieciski, K. Krasnowski, K., Jachym, R. (2009). Characteristics of Nd: YAG laser welded joints of dual phase steel. Archives of civil and mechanical engineering, Vol. IX No. 4. (8) Padmanaban, G. and Balasubramanian, V. (2010). An Optimization of laser beam welding process parameters to attain maximum tensile strength in AZ31B magnesium alloy Optics & Laser Technology 42 (2010) 1253–1260. (9) Sathiya, P., Panneerselvam, K. and Soundararajan, R. (2010). Optimal design for laser beam butt welding process parameter using artificial neural networks and genetic algorithm for super austenitic stainless steel / Optics & Laser Technology 44.1905–1914 (10) Minitab 16 software for quality improvement by MINITAB (11) A Hussain, A H Hamdani and R Akhter 1 Pakistan Institute of Lasers & Optics, P.O. Box 505, Rawalpindi, Pakistan (12) Klimpel A and Lisiecki A 2007 J. Achiev. Mater. and Manuf. Eng. Vol. 25 1.
© 2018, IRJET

Impact Factor value: 7.211

ISO 9001:2008 Certified Journal

Page 2982
https://www.irjet.net/archives/V5/i6/IRJETV5I6571.pdf
Published on Aug 10, 2018
https://www.irjet.net/archives/V5/i6/IRJETV5I6571.pdf